Cadmium selenite‒water (4/3) and two polymorphic forms of cadmium selenite
Valkonen, J.; Acta Crystallographica Section C 50 (1994) 991–994; doi:10.1107/S0108270193011278

data_2009817
_publ_section_title
;
 Cadmium selenite--water (4/3) and two polymorphic forms of cadmium
 selenite
;
_journal_issue                   7
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              991
_journal_page_last               994
_journal_paper_doi               10.1107/S0108270193011278
_journal_volume                  50
_journal_year                    1994
_chemical_formula_sum            'Cd O3 Se'
_chemical_formula_weight         239.36
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_type_scat_source           'IntTabIV Tables 2.2B and 2.3.1'
_cell_angle_alpha                90.
_cell_angle_beta                 101.210(8)
_cell_angle_gamma                90.
_cell_formula_units_Z            8
_cell_length_a                   5.7084(5)
_cell_length_b                   12.8283(11)
_cell_length_c                   8.5860(8)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    298
_cell_measurement_theta_max      12.15
_cell_measurement_theta_min      7.99
_cell_volume                     616.75(10)
_diffrn_measurement_device       'Enraf-Nonius CAD-4'
_diffrn_measurement_method       2\q/\w
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            3946
_diffrn_reflns_theta_max         39.98
_diffrn_standards_decay_%        <2
_diffrn_standards_interval_time  60
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    18.54
_exptl_absorpt_correction_T_max  1.091
_exptl_absorpt_correction_T_min  0.900
_exptl_absorpt_correction_type   DIFABS
_exptl_crystal_colour            white
_exptl_crystal_density_diffrn    5.16
_exptl_crystal_description       prismatic
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.10
_refine_diff_density_max         3.12
_refine_diff_density_min         -4.39
_refine_ls_extinction_coef       'g = 5.60x10^-7^'
_refine_ls_extinction_method
'|F~c~| +|F~o~|x(1+gIc) (Stout & Jenson, 1968)'
_refine_ls_goodness_of_fit_obs   4.36
_refine_ls_number_parameters     92
_refine_ls_number_reflns         2862
_refine_ls_R_factor_obs          4.3
_refine_ls_shift/esd_max         0.005
_refine_ls_structure_factor_coef F
_refine_ls_weighting_scheme      unit
_refine_ls_wR_factor_obs         6.2
_reflns_number_observed          2862
_reflns_number_total             3946
_reflns_observed_criterion       I>3\s(I)
_cod_data_source_file            ab1066.cif
_cod_data_source_block           ab1066_structure_2_of_3
_cod_original_cell_volume        616.70(10)
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_original_formula_sum        'Cd1 O3 Se1'
_cod_database_code               2009817